LMucko/crystallography-open-database huggingface dataset:
Mossbauer studies of thiospinels. V. The systems Cu1-xFexMe2S4 (Me=Cr,Rh) and Cu1-xFexCr2(S.7Se.3)4 Locality: synthetic
Riedel, E.; Karl, R.; Rackwitz, R.; Journal of Solid State Chemistry 40 (1981) 255–265; doi:10.1016/0022-4596(81)90390-X

data_9012170
_publ_section_title
;Mossbauer studies of thiospinels. V. The systems Cu1-xFexMe2S4 (Me=Cr,Rh) and
 Cu1-xFexCr2(S.7Se.3)4 Locality: synthetic
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              255
_journal_page_last               265
_journal_paper_doi               10.1016/0022-4596(81)90390-X
_journal_volume                  40
_journal_year                    1981
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Cr2 Cu0.45 Fe0.55 S2.8 Se1.2'
_chemical_name_mineral           Daubreelite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   10.063
_cell_length_b                   10.063
_cell_length_c                   10.063
_cell_formula_units_Z            8
_cell_volume                     1019.019
_database_code_amcsd             0013451
_exptl_crystal_density_diffrn    4.535
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Cu.45 Fe.55) Cr2 (S2.8 Se1.2)'
_cod_database_code               9012170
Mossbauer studies of thiospinels. V. The systems Cu1-xFexMe2S4 (Me=Cr,Rh) and Cu1-xFexCr2(S.7Se.3)4 Locality: synthetic
Riedel, E.; Karl, R.; Rackwitz, R.; Journal of Solid State Chemistry 40 (1981) 255–265; doi:10.1016/0022-4596(81)90390-X

data_9012171
_publ_section_title
;Mossbauer studies of thiospinels. V. The systems Cu1-xFexMe2S4 (Me=Cr,Rh) and
 Cu1-xFexCr2(S.7Se.3)4 Locality: synthetic
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              255
_journal_page_last               265
_journal_paper_doi               10.1016/0022-4596(81)90390-X
_journal_volume                  40
_journal_year                    1981
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Cr2 Cu0.4 Fe0.6 S2.8 Se1.2'
_chemical_name_mineral           Daubreelite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   10.072
_cell_length_b                   10.072
_cell_length_c                   10.072
_cell_formula_units_Z            8
_cell_volume                     1021.756
_database_code_amcsd             0013452
_exptl_crystal_density_diffrn    4.517
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Cu.4 Fe.6) Cr2 (S2.8 Se1.2)'
_cod_database_code               9012171
Mossbauer studies of thiospinels. V. The systems Cu1-xFexMe2S4 (Me=Cr,Rh) and Cu1-xFexCr2(S.7Se.3)4 Locality: synthetic
Riedel, E.; Karl, R.; Rackwitz, R.; Journal of Solid State Chemistry 40 (1981) 255–265; doi:10.1016/0022-4596(81)90390-X

data_9012172
_publ_section_title
;Mossbauer studies of thiospinels. V. The systems Cu1-xFexMe2S4 (Me=Cr,Rh) and
 Cu1-xFexCr2(S.7Se.3)4 Locality: synthetic
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              255
_journal_page_last               265
_journal_paper_doi               10.1016/0022-4596(81)90390-X
_journal_volume                  40
_journal_year                    1981
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Cr2 Cu0.35 Fe0.65 S2.8 Se1.2'
_chemical_name_mineral           Daubreelite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   10.081
_cell_length_b                   10.081
_cell_length_c                   10.081
_cell_formula_units_Z            8
_cell_volume                     1024.497
_database_code_amcsd             0013453
_exptl_crystal_density_diffrn    4.500
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Cu.35 Fe.65) Cr2 (S2.8 Se1.2)'
_cod_database_code               9012172
Mossbauer studies of thiospinels. V. The systems Cu1-xFexMe2S4 (Me=Cr,Rh) and Cu1-xFexCr2(S.7Se.3)4 Locality: synthetic
Riedel, E.; Karl, R.; Rackwitz, R.; Journal of Solid State Chemistry 40 (1981) 255–265; doi:10.1016/0022-4596(81)90390-X

data_9012173
_publ_section_title
;Mossbauer studies of thiospinels. V. The systems Cu1-xFexMe2S4 (Me=Cr,Rh) and
 Cu1-xFexCr2(S.7Se.3)4 Locality: synthetic
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              255
_journal_page_last               265
_journal_paper_doi               10.1016/0022-4596(81)90390-X
_journal_volume                  40
_journal_year                    1981
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Cr2 Cu0.3 Fe0.7 S2.8 Se1.2'
_chemical_name_mineral           Daubreelite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   10.091
_cell_length_b                   10.091
_cell_length_c                   10.091
_cell_formula_units_Z            8
_cell_volume                     1027.549
_database_code_amcsd             0013454
_exptl_crystal_density_diffrn    4.482
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Cu.3 Fe.7) Cr2 (S2.8 Se1.2)'
_cod_database_code               9012173
Mossbauer studies of thiospinels. V. The systems Cu1-xFexMe2S4 (Me=Cr,Rh) and Cu1-xFexCr2(S.7Se.3)4 Locality: synthetic
Riedel, E.; Karl, R.; Rackwitz, R.; Journal of Solid State Chemistry 40 (1981) 255–265; doi:10.1016/0022-4596(81)90390-X

data_9012174
_publ_section_title
;Mossbauer studies of thiospinels. V. The systems Cu1-xFexMe2S4 (Me=Cr,Rh) and
 Cu1-xFexCr2(S.7Se.3)4 Locality: synthetic
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              255
_journal_page_last               265
_journal_paper_doi               10.1016/0022-4596(81)90390-X
_journal_volume                  40
_journal_year                    1981
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Cr2 Cu0.2 Fe0.8 S2.8 Se1.2'
_chemical_name_mineral           Daubreelite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   10.103
_cell_length_b                   10.103
_cell_length_c                   10.103
_cell_formula_units_Z            8
_cell_volume                     1031.219
_database_code_amcsd             0013455
_exptl_crystal_density_diffrn    4.456
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Cu.2 Fe.8) Cr2 (S2.8 Se1.2)'
_cod_database_code               9012174
Mossbauer studies of thiospinels. V. The systems Cu1-xFexMe2S4 (Me=Cr,Rh) and Cu1-xFexCr2(S.7Se.3)4 Locality: synthetic
Riedel, E.; Karl, R.; Rackwitz, R.; Journal of Solid State Chemistry 40 (1981) 255–265; doi:10.1016/0022-4596(81)90390-X

data_9012175
_publ_section_title
;Mossbauer studies of thiospinels. V. The systems Cu1-xFexMe2S4 (Me=Cr,Rh) and
 Cu1-xFexCr2(S.7Se.3)4 Locality: synthetic
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              255
_journal_page_last               265
_journal_paper_doi               10.1016/0022-4596(81)90390-X
_journal_volume                  40
_journal_year                    1981
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Cr2 Cu0.1 Fe0.9 S2.8 Se1.2'
_chemical_name_mineral           Daubreelite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   10.122
_cell_length_b                   10.122
_cell_length_c                   10.122
_cell_formula_units_Z            8
_cell_volume                     1037.048
_database_code_amcsd             0013456
_exptl_crystal_density_diffrn    4.421
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Cu.1 Fe.9) Cr2 (S2.8 Se1.2)'
_cod_database_code               9012175
Mossbauer studies of thiospinels. V. The systems Cu1-xFexMe2S4 (Me=Cr,Rh) and Cu1-xFexCr2(S.7Se.3)4 Locality: synthetic
Riedel, E.; Karl, R.; Rackwitz, R.; Journal of Solid State Chemistry 40 (1981) 255–265; doi:10.1016/0022-4596(81)90390-X

data_9012176
_publ_section_title
;Mossbauer studies of thiospinels. V. The systems Cu1-xFexMe2S4 (Me=Cr,Rh) and
 Cu1-xFexCr2(S.7Se.3)4 Locality: synthetic
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              255
_journal_page_last               265
_journal_paper_doi               10.1016/0022-4596(81)90390-X
_journal_volume                  40
_journal_year                    1981
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Cr2 Fe S2.8 Se1.2'
_chemical_name_mineral           Daubreelite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   10.136
_cell_length_b                   10.136
_cell_length_c                   10.136
_cell_formula_units_Z            8
_cell_volume                     1041.357
_database_code_amcsd             0013457
_exptl_crystal_density_diffrn    4.393
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Fe Cr2 (S2.8 Se1.2)'
_cod_database_code               9012176
What is the true space group of weberite? Sample: Imma refinement, T = ambient
Knop, O.; Cameron, T. S.; Jochem, K.; Journal of Solid State Chemistry 43 (1982) 213–221; doi:10.1016/0022-4596(82)90231-6

data_9012177
_publ_section_title
;
 What is the true space group of weberite?
 Sample: Imma refinement, T = ambient
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              213
_journal_page_last               221
_journal_paper_doi               10.1016/0022-4596(82)90231-6
_journal_volume                  43
_journal_year                    1982
_chemical_compound_source        'Ivigtut, Greenland'
_chemical_formula_sum            'Al F7 Mg Na2'
_chemical_name_mineral           Weberite
_symmetry_space_group_name_H-M   'I m m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.051
_cell_length_b                   9.968
_cell_length_c                   7.285
_cell_formula_units_Z            4
_cell_volume                     512.022
_database_code_amcsd             0013477
_exptl_crystal_density_diffrn    2.987
_cod_original_formula_sum        'Na2 Mg Al F7'
_cod_database_code               9012177
What is the true space group of weberite? Sample: Imma refinement, T = 133 K
Knop, O.; Cameron, T. S.; Jochem, K.; Journal of Solid State Chemistry 43 (1982) 213–221; doi:10.1016/0022-4596(82)90231-6

data_9012178
_publ_section_title
;
 What is the true space group of weberite?
 Sample: Imma refinement, T = 133 K
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              213
_journal_page_last               221
_journal_paper_doi               10.1016/0022-4596(82)90231-6
_journal_volume                  43
_journal_year                    1982
_chemical_compound_source        'Ivigtut, Greenland'
_chemical_formula_sum            'Al F7 Mg Na2'
_chemical_name_mineral           Weberite
_symmetry_space_group_name_H-M   'I m m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.050
_cell_length_b                   9.979
_cell_length_c                   7.297
_cell_formula_units_Z            4
_cell_volume                     513.358
_database_code_amcsd             0013478
_diffrn_ambient_temperature      133
_exptl_crystal_density_diffrn    2.979
_cod_original_formula_sum        'Na2 Mg Al F7'
_cod_database_code               9012178
What is the true space group of weberite? Sample: Imm2 refinement, T = ambient
Knop, O.; Cameron, T. S.; Jochem, K.; Journal of Solid State Chemistry 43 (1982) 213–221; doi:10.1016/0022-4596(82)90231-6

data_9012179
_publ_section_title
;
 What is the true space group of weberite?
 Sample: Imm2 refinement, T = ambient
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              213
_journal_page_last               221
_journal_paper_doi               10.1016/0022-4596(82)90231-6
_journal_volume                  43
_journal_year                    1982
_chemical_compound_source        'Ivigtut, Greenland'
_chemical_formula_sum            'Al F7 Mg Na2'
_chemical_name_mineral           Weberite
_space_group_IT_number           44
_symmetry_space_group_name_Hall  'I 2 -2'
_symmetry_space_group_name_H-M   'I m m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.051
_cell_length_b                   9.968
_cell_length_c                   7.285
_cell_formula_units_Z            4
_cell_volume                     512.022
_database_code_amcsd             0013479
_exptl_crystal_density_diffrn    2.987
_cod_original_formula_sum        'Na2 Mg Al F7'
_cod_database_code               9012179
What is the true space group of weberite? Sample: Imm2 refinement, T = 133 K
Knop, O.; Cameron, T. S.; Jochem, K.; Journal of Solid State Chemistry 43 (1982) 213–221; doi:10.1016/0022-4596(82)90231-6

data_9012180
_publ_section_title
;
 What is the true space group of weberite?
 Sample: Imm2 refinement, T = 133 K
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              213
_journal_page_last               221
_journal_paper_doi               10.1016/0022-4596(82)90231-6
_journal_volume                  43
_journal_year                    1982
_chemical_compound_source        'Ivigtut, Greenland'
_chemical_formula_sum            'Al F7 Mg Na2'
_chemical_name_mineral           Weberite
_space_group_IT_number           44
_symmetry_space_group_name_Hall  'I 2 -2'
_symmetry_space_group_name_H-M   'I m m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.050
_cell_length_b                   9.979
_cell_length_c                   7.297
_cell_formula_units_Z            4
_cell_volume                     513.358
_database_code_amcsd             0013480
_diffrn_ambient_temperature      133
_exptl_crystal_density_diffrn    2.979
_cod_original_formula_sum        'Na2 Mg Al F7'
_cod_database_code               9012180
What is the true space group of weberite? Sample: I2_12_12_1 refinement, T = ambient Note: y(F6) and z(F6) corrected
Knop, O.; Cameron, T. S.; Jochem, K.; Journal of Solid State Chemistry 43 (1982) 213–221; doi:10.1016/0022-4596(82)90231-6

data_9012181
_publ_section_title
;
 What is the true space group of weberite?
 Sample: I2_12_12_1 refinement, T = ambient
 Note: y(F6) and z(F6) corrected
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              213
_journal_page_last               221
_journal_paper_doi               10.1016/0022-4596(82)90231-6
_journal_volume                  43
_journal_year                    1982
_chemical_compound_source        'Ivigtut, Greenland'
_chemical_formula_sum            'Al F7 Mg Na2'
_chemical_name_mineral           Weberite
_symmetry_space_group_name_H-M   'I 21 21 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.051
_cell_length_b                   9.968
_cell_length_c                   7.285
_cell_formula_units_Z            4
_cell_volume                     512.022
_database_code_amcsd             0013481
_exptl_crystal_density_diffrn    2.987
_cod_original_formula_sum        'Na2 Mg Al F7'
_cod_database_code               9012181
What is the true space group of weberite? Sample: I2_12_12_1 refinement, T = 133 K Note: y(F6) and z(F6) corrected
Knop, O.; Cameron, T. S.; Jochem, K.; Journal of Solid State Chemistry 43 (1982) 213–221; doi:10.1016/0022-4596(82)90231-6

data_9012182
_publ_section_title
;
 What is the true space group of weberite?
 Sample: I2_12_12_1 refinement, T = 133 K
 Note: y(F6) and z(F6) corrected
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              213
_journal_page_last               221
_journal_paper_doi               10.1016/0022-4596(82)90231-6
_journal_volume                  43
_journal_year                    1982
_chemical_compound_source        'Ivigtut, Greenland'
_chemical_formula_sum            'Al F7 Mg Na2'
_chemical_name_mineral           Weberite
_symmetry_space_group_name_H-M   'I 21 21 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.050
_cell_length_b                   9.979
_cell_length_c                   7.297
_cell_formula_units_Z            4
_cell_volume                     513.358
_database_code_amcsd             0013482
_diffrn_ambient_temperature      133
_exptl_crystal_density_diffrn    2.979
_cod_original_formula_sum        'Na2 Mg Al F7'
_cod_database_code               9012182
What is the true space group of weberite? Sample: I2mb refinement, T = ambient Note: z(F6) corrected
Knop, O.; Cameron, T. S.; Jochem, K.; Journal of Solid State Chemistry 43 (1982) 213–221; doi:10.1016/0022-4596(82)90231-6

data_9012183
_publ_section_title
;
 What is the true space group of weberite?
 Sample: I2mb refinement, T = ambient
 Note: z(F6) corrected
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              213
_journal_page_last               221
_journal_paper_doi               10.1016/0022-4596(82)90231-6
_journal_volume                  43
_journal_year                    1982
_chemical_compound_source        'Ivigtut, Greenland'
_chemical_formula_sum            'Al F7 Mg Na2'
_chemical_name_mineral           Weberite
_symmetry_space_group_name_H-M   'I 2 m b'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.051
_cell_length_b                   9.968
_cell_length_c                   7.285
_cell_formula_units_Z            4
_cell_volume                     512.022
_database_code_amcsd             0013483
_exptl_crystal_density_diffrn    2.987
_cod_original_formula_sum        'Na2 Mg Al F7'
_cod_database_code               9012183
What is the true space group of weberite? Sample: I2mb refinement, T = 133 K Note: z(F6) corrected
Knop, O.; Cameron, T. S.; Jochem, K.; Journal of Solid State Chemistry 43 (1982) 213–221; doi:10.1016/0022-4596(82)90231-6

data_9012184
_publ_section_title
;
 What is the true space group of weberite?
 Sample: I2mb refinement, T = 133 K
 Note: z(F6) corrected
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              213
_journal_page_last               221
_journal_paper_doi               10.1016/0022-4596(82)90231-6
_journal_volume                  43
_journal_year                    1982
_chemical_compound_source        'Ivigtut, Greenland'
_chemical_formula_sum            'Al F7 Mg Na2'
_chemical_name_mineral           Weberite
_symmetry_space_group_name_H-M   'I 2 m b'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   7.051
_cell_length_b                   9.968
_cell_length_c                   7.285
_cell_formula_units_Z            4
_cell_volume                     512.022
_database_code_amcsd             0013484
_diffrn_ambient_temperature      133
_exptl_crystal_density_diffrn    2.987
_cod_original_formula_sum        'Na2 Mg Al F7'
_cod_database_code               9012184
The crystal structure of tveitite, an ordered yttrofluorite mineral Note: a and b adjusted to match reported bond lengths
Bevan, D. J. M.; Strahle, J.; Greis, O.; Journal of Solid State Chemistry 44 (1982) 75–81; doi:10.1016/0022-4596(82)90402-9

data_9012185
_publ_section_title
;
 The crystal structure of tveitite, an ordered yttrofluorite mineral
 Note: a and b adjusted to match reported bond lengths
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              75
_journal_page_last               81
_journal_paper_doi               10.1016/0022-4596(82)90402-9
_journal_volume                  44
_journal_year                    1982
_chemical_formula_sum            'Ca6.5 F21.5 Y3'
_chemical_name_mineral           Tveitite-(Y)
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   16.9620
_cell_length_b                   16.9620
_cell_length_c                   9.6664
_cell_formula_units_Z            6
_cell_volume                     2408.516
_database_code_amcsd             0013486
_exptl_crystal_density_diffrn    3.871
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        'Y3 Ca6.5 F21.5'
_cod_database_code               9012185
Fe3PO7, un cas de coordinence 5 du fer trivalent, etude structurale et magnetique Locality: synthetic
Modaressi, A.; Courtois, A.; Gerardin, R.; Malaman, B.; Gleitzer, C.; Journal of Solid State Chemistry 47 (1983) 245–255; doi:10.1016/0022-4596(83)90016-6

data_9012186
_publ_section_title
;Fe3PO7, un cas de coordinence 5 du fer trivalent, etude structurale et
 magnetique Locality: synthetic
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              245
_journal_page_last               255
_journal_paper_doi               10.1016/0022-4596(83)90016-6
_journal_volume                  47
_journal_year                    1983
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe3 O7 P'
_chemical_name_mineral           Grattarolaite
_space_group_IT_number           160
_symmetry_space_group_name_Hall  'R 3 -2"'
_symmetry_space_group_name_H-M   'R 3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   8.006
_cell_length_b                   8.006
_cell_length_c                   6.863
_cell_formula_units_Z            3
_cell_volume                     380.957
_database_code_amcsd             0013505
_exptl_crystal_density_diffrn    4.060
_cod_original_sg_symbol_H-M      'R 3 m'
_cod_original_formula_sum        'Fe3 P O7'
_cod_database_code               9012186